Lecture 22: Spinodal Decomposition: Part 1: general description and


 Teresa Ball
 1 years ago
 Views:
Transcription
1 Lecture 22: Spinodal Decomposition: Part 1: general description and practical implications Today s topics basics and unique features of spinodal decomposition and its practical implications. The relationship between the phase diagram and the free energy ( G) vs. composition plot. Initial understanding of spinodal decomposition from the CahnHilliard Equation. About Spinodal decomposition Spinodal decomposition is a mechanism by which a solution of two or more components can separate into distinct phases with distinctly different chemical compositions and physical properties. This mechanism differs from the classical nucleation (as we went through in previous Lectures #1014): the phase separation due to spinodal decomposition is much more defined, and occurs uniformly throughout the material not just at discrete nucleation sites. (see an animation for the microstructural evolution under the Cahn Hilliard equation, demonstrating distinctive coarsening and phase separation through spinodal decomposition: and also a movie clip simulating the phase separation due to spinodal decomposition on a hexagonal lattice (from Oono, Y. and Puri, S., Study of phaseseparation dynamics by use of cell dynamical systems. I. Modeling, Physical Review A (General Physics), Volume 38, Issue 1, July 1, 1988, pp ): Spinodal decomposition is of interest primarily due to its inherent simplicity, and thus represents one of the few phase transformations in solids for which there is any plausible quantitative theory. Since there is no thermodynamic barrier to the reaction inside of the spinodal region, the decomposition is determined solely by diffusion. Thus, the process can be treated purely as a diffusion problem, and many of the characteristics of the decomposition can be described by an approximate analytical solution to the general diffusion equation. In contrast, theories of nucleation and growth have to invoke the thermodynamics of fluctuations, and the diffusion problem involved in the growth of the nucleus is far more difficult to solve, because it is unrealistic to linearize the diffusion equation. Spinodal decomposition is also of interest from a more practical standpoint, as it provides a means of producing a very finely dispersed microstructure that can significantly enhance the physical properties of the material. A lot of examples of materials in real practice require such defined phase segregation. One example is the plastic solar cells 1
2 (see picture below), where the C60 and polymer phase should be well separated to provide separate charge carrier transport thus minimizing the charge recombination, but meanwhile still maintaining the large interface contact to maximize the photoinduced charge separation to produce the free charge carriers (electrons and holes), which in turn demands uniform, very finely dispersed micro or even nanoscale structured phases of the ntype and ptype materials. To this end, the smaller the segregation (the wavelength, λ, as to be described below), the large the interface, and thus the more the np contact, and thus the more efficient for the photoinduced charge separation. Plastic solar cell device based on a sanwiched compsoiteds of conducting polymer and C60: In (a) both the polymer nanospheres as well as the fullerene phase offer percolated pathways for the transport of holes and electrons, respectively. In (b) electrons and holes suffer recombination, as the percolation is not sufficient. High resolution TEM images of regioregular polymer:c60 (P3HT:PCBM 1:0.8) blend films cast from chlorobenzene, (a) as cast, (b) annealed at 150 C for 30 min and (c) for 2 hours. Clearly visible are the spherical P3HT nanostructures with a size on the order of 10 nm. Several Important Terms: Miscibility Gap: Area within the coexistence curve of an isobaric phase diagram (temperature vs composition) or an isothermal phase diagram (pressure vs. composition). A miscibility gap is observed at temperatures below an upper critical solution temperature (UCST) or above the lower critical solution 2
3 temperature (LCST). Its location depends on pressure. In the miscibility gap, there are at least two phases coexisting. Below is an example of LiquidLiquid Equilibrium (Miscibility Gap) Mixture of Ethanol and Dodecane. Binodal Curve or Coexistence Curve: It is a curve (like the belllike one shown above) defining the region of composition and temperature in a phase diagram for a binary mixture across which a transition occurs from miscibility of the components to conditions where singlephase mixtures are metastable or unstable. Binodal compositions are defined by pairs of points on the curve of Gibbs energy of mixing vs composition that have common tangents, corresponding to compositions of equal chemical potentials of each of the two components in two phases. Spinodal Curve: A curve that separates a metastable region from an unstable region in the coexistence region of a binary mixture. Above the spinodal curve the process of moving towards equilibrium occurs by droplet nucleation, while below the spinodal curve there are periodic modulations of the order parameter, which have a small amplitude at first (i.e., spinodal decomposition). Spinodal curve is not a sharp boundary in real systems as a result of fluctuations. Phase Diagram and Freeenergy Diagram of spinodal decomposition: As a special case of phase transformation, spinodal decomposition can be illustrated on a phase diagram exhibiting a miscibility gap (see the diagram below). Thus, phase separation occurs whenever a material transitions into the unstable region of the phase diagram. The boundary of the unstable region, sometimes referred to as the binodal or coexistence curve, is found by performing a common tangent construction of the freeenergy diagram. Inside the binodal is a region called the spinodal, which is found by determining 3
4 where the curvature of the freeenergy curve is negative. The binodal and spinodal meet at the critical point. It is when a material is moved into the spinodal region of the phase diagram that spinodal decomposition can occur. If an alloy with composition of X 0 is solution treated at a high temperature T 1, and then quenched (rapidly cooled) to a lower temperature T 2, the composition will initially be the same everywhere and its free energy will be G 0 on the G curve in the following diagram. However, the alloy will be immediately unstable, because small fluctuation in composition that produces Arich and Brich regions will cause the total free energy to decrease. Therefore, uphill diffusion (see the illustration at the end of this lecture) takes place until the equilibrium compositions X 1 and X 2 are reached. How such small composition fluctuation leads to the spinodal phase separation is today s and next two lectures topics. In comparison, if an alloy lies outside the spinodal (i.e., with composition of X 0 as shown) is solution treated at a high temperature T 1, and then quenched to a lower temperature T 2, small variations in composition lead to an increase in free energy (as shown), and the alloy is therefore metastable. The free energy of the system cam only be decreased in this case if nuclei are formed with a composition very different from the matrix. Therefore outside the spinodal the transformation must proceed by a process of nucleation and growth as we learned in the past Lectures d 2 G/dc 2 < 0 c or X here refers to the concentration of components. adapted from the Book "Phase Transformations in Metals and Alloys", by D. A. Porter, K. E. Easterling and M. Y. Sherif, CRC Press, third edition. 4
5 The free energy curve is plotted as a function of composition for the phase separation temperature T 2. Equilibrium phase compositions are those corresponding to the free energy minima. Regions of negative curvature (d 2 G/dc 2 < 0 ) lie within the inflection points of the curve (d 2 G/dc 2 = 0 ) which are called the spinodes (as marked as S 1 and S 2 in the diagram above). For compositions within the spinodal, a homogeneous solution is unstable against microscopic fluctuations in density or composition, and there is no thermodynamic barrier to the growth of a new phase, i.e., the phase transformation is solely diffusion controlled. To reach the spinodal region of the phase diagram, a transition must take the material through the binodal region or the critical point. Often phase separation will occur via nucleation during this transition, and spinodal decomposition will not be observed. To observe spinodal decomposition, a very fast transition, often called a quench, is required to move from the stable to the spinodally unstable region of the phase diagram. Brief description of Spinodal Decomposition following the Freeenergy Diagram Spinodal decomposition is a mechanism by which a solution of two or more components can separate into distinct phases with distinctly different chemical compositions and physical properties. This mechanism differs from the classical nucleation (as we went through in previous Lectures #1014 ): the phase separation due to spinodal decomposition is much more defined, and occurs uniformly throughout the material not just at discrete nucleation sites. Spinodal decomposition is also of interest from a more practical standpoint, as it provides a means of producing a very finely dispersed microstructure that can significantly enhance the physical properties of the material. As a special case of phase transformation, spinodal decomposition can be illustrated on a phase diagram exhibiting a miscibility gap (see the diagram below). Thus, phase separation occurs whenever a material transitions into the unstable region of the phase diagram. The boundary of the unstable region, sometimes referred to as the binodal or coexistence curve, is found by performing a common tangent construction of the freeenergy diagram. Inside the binodal is a region called the spinodal, which is found by determining where the curvature of the freeenergy curve is negative. The binodal and spinodal meet at the critical point. It is when a material is moved into the spinodal region of the phase diagram that spinodal decomposition can occur. If an alloy with composition of X 0 is solution treated at a high temperature T 1, and then quenched (rapidly cooled) to a lower temperature T 2, the composition will initially be the same everywhere and its free energy will be G 0 on the G curve in the following diagram. However, the alloy will be immediately unstable, because small fluctuation in composition that produces Arich and Brich regions will cause the total free energy to decrease. Therefore, uphill diffusion (as shown) takes place until the equilibrium compositions X 1 and X 2 are reached. How such small composition fluctuation leads to the spinodal phase separation is today s and next two lectures topics. In comparison, if an alloy lies outside the spinodal (i.e., with composition of X 0 as shown) is solution treated at a high temperature T 1, and then quenched to a lower temperature T 2, small variations in 5
6 composition lead to an increase in free energy (as shown), and the alloy is therefore metastable. The free energy of the system cam only be decreased in this case if nuclei are formed with a composition very different from the matrix. Therefore outside the spinodal the transformation must proceed by a process of nucleation and growth as we learned in the past Lectures The free energy curve is plotted as a function of composition for the phase separation temperature T 2. Equilibrium phase compositions are those corresponding to the free energy minima. Regions of negative curvature (d 2 G/dc 2 < 0 ) lie within the inflection points of the curve (d 2 G/dc 2 = 0 ) which are called the spinodes (as marked as S 1 and S 2 in the diagram above). For compositions within the spinodal, a homogeneous solution is unstable against microscopic fluctuations in density or composition, and there is no thermodynamic barrier to the growth of a new phase, i.e., the phase transformation is solely diffusion controlled. Early Background of Spinodal Decomposition: In the early 1940s, Bradley reported the observation of sidebands around the Bragg peaks of the xray diffraction pattern from a CuNiFe alloy that had been quenched and then annealed inside the miscibility gap. Further observations on the same alloy were made by Daniel and Lipson, who demonstrated that the sidebands could be explained by a periodic modulation of composition in the <100> directions. From the spacing of the sidebands they were able to determine the wavelength of the modulation, which was of the order of 100 Å. The growth of a composition modulation in an initially homogeneous alloy implies uphill diffusion (see the illustration at the end of this lecture), or a negative diffusion coefficient (see Lecture 5). Becker and Dehlinger had already predicted a negative diffusivity inside the spinodal region of a binary system. But their treatments could not account for the growth of a modulation of particular wavelength (λ), such as was observed in the CuNiFe alloy. In fact, any model based on Fick's law yields a physically unacceptable solution when the diffusion coefficient is negative (see Lecture 5). The first explanation of the periodicity was given by Mats Hillert in his 1955 Doctoral Dissertation at MIT. Starting with a regular solution model, he derived a flux equation for onedimensional diffusion on a discrete lattice. This equation differed from the usual one by the inclusion of a term which allowed for the effect on the driving force of the interfacial energy between adjacent interatomic planes that differed in composition. Hillert solved the flux equation numerically and found that inside the spinodal it yielded a periodic variation of composition with distance. Furthermore, the wavelength of the modulation was of the same order as that observed in the CuNiFe alloys. A more flexible continuum model was subsequently developed by John W. Cahn, who included the effects of coherency strains as well as the gradient energy term. The strains are significant in that they dictate the ultimate morphology of the decomposition in anisotropic materials. About Mats Hillert: Mats Hillert, born November 28, 1924 in Gothenburg, is a Swedish metallurgist who is an emeritus professor in metallography (physical 6
7 metallurgy) at the Royal Institute of Technology (KTH). Hillert has made contribution to many areas of metals research, including thermodynamics and phase transitions. In 1973, he was elected a member of the Royal Swedish Academy of Engineering Sciences, and in 1982 a member of the Royal Swedish Academy of Sciences. About John W. Cahn: John Werner Cahn (born 1928) is an American scientist and winner of the National Medal of Science in Since 1977, he has held a position at the National Institute of Standards and Technolog. Cahn received a bachelor's degree in Chemistry in 1949 from the University of Michigan. He later earned a Ph.D in Physical Chemistry in 1953 from the University of California at Berkeley Member, National Academy of Sciences Member, National Academy of Engineering Comparison between Spinodal Decomposition and Nucleation and Growth An initially homogeneous solution develops fluctuations of chemical composition when supercooled into the spinodal region. These fluctuations are at first small in amplitude but grow with time until there are identifiable precipitates of equilibrium composition (vide infra). In contrast, during nucleation and growth, there is a sharp interface between the parent and product crystals; furthermore, the precipitate at all stages of its existence has the required equilibrium composition (vide infra). Spinodal decomposition involves uphill diffusion, whereas diffusion is always down a concentration gradient for nucleation and growth of the type illustrated below. Spinodal decomposition refers to a mechanism of phase transformation inside a miscibility gap. It is characterized by the occurrence of diffusion up against a concentration gradient (see Lecture 5), often referred as uphill diffusion (see the illustration at the end of this lecture), leading to formation of a uniformsized, periodic fine microstructure. 7
8 Illustration: Evolution of phase separation in spinodal decomposition and during nucleation and growth. The arrows indicate the direction of diffusion.  from Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia, Cambridge U. 8
Lecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More information4. Thermodynamics of Polymer Blends
4. Thermodynamics of Polymer Blends Polymeric materials find growing applications in various fields of everyday life because they offer a wide range of application relevant properties. Blending of polymers
More informationPhase Diagrams and Phase Separation. MF Ashby and DA Jones, Engineering Materials Vol 2, Pergamon. G Strobl, The Physics of Polymers, Springer
and Phase Separation Books MF Ashby and DA Jones, Engineering Materials Vol 2, Pergamon P Haasen, Physical Metallurgy, G Strobl, The Physics of Polymers, Springer Introduction Mixing two (or more) components
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More informationMark Asta Mat Sci 103 Spring, 2016 mdasta@berkeley.edu Phase Transformations & Kinetics LOGISTICS
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering Mark Asta Mat Sci 103 Spring, 2016 mdasta@berkeley.edu Phase Transformations & Kinetics LOGISTICS Course Website
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationLecture: 33. Solidification of Weld Metal
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationRAPIDLY SOLIDIFIED COPPER ALLOYS RIBBONS
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.35153.881412.2=20 RAPIDLY SOLIDIFIED COPPER ALLOYS RIBBONS M. ŠULER 1, L. KOSEC 1, A. C. KNEISSL 2, M. BIZJAK 1, K. RAIĆ
More informationApplication of image analysis for characterization of powders
Materials SciencePoland, Vol. 23, No. 1, 2005 Application of image analysis for characterization of powders JAKUB MICHALSKI 1*, TOMASZ WEJRZANOWSKI 1, ROMAN PIELASZEK 2, KATARZYNA KONOPKA 1, WITOLD ŁOJKOWSKI
More informationLecture 24: Spinodal Decomposition: Part 3: kinetics of the
Leture 4: Spinodal Deoposition: Part 3: kinetis of the oposition flutuation Today s topis Diffusion kinetis of spinodal deoposition in ters of the onentration (oposition) flutuation as a funtion of tie:
More informationEffect of Temperature and Aging Time on 2024 Aluminum Behavior
Proceedings of the XIth International Congress and Exposition June 25, 2008 Orlando, Florida USA 2008 Society for Experimental Mechanics Inc. Effect of Temperature and Aging Time on 2024 Aluminum Behavior
More information5 Some standard heat treatments
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
More informationThe ClausiusClapeyron Equation:
Chapter 10 Solid Solutions and Phase Equilibrium What is a phase? Phase Diagram Basics A phase diagram represents what phases are present at a given pressure, temperature and composition. Virtual maps
More informationLecture 3: Models of Solutions
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP4, Thermodynamics and Phase Diagrams, H. K. D. H. Bhadeshia Lecture 3: Models of Solutions List of Symbols Symbol G M
More informationIntroduction to XRay Powder Diffraction Data Analysis
Introduction to XRay Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An Xray diffraction pattern is a plot of the intensity of Xrays scattered
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationMean Field Flory Huggins Lattice Theory
Mean Field Flory Huggins Lattice Theory Mean field: the interactions between molecules are assumed to be due to the interaction of a given molecule and an average field due to all the other molecules in
More informationMartensite in Steels
Materials Science & Metallurgy http://www.msm.cam.ac.uk/phasetrans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationStudy on the Mechanism of Strengthening and Toughening Effect of Titanium Addition on HSLA Steel
Study on the Mechanism of Strengthening and Toughening Effect of Titanium Addition on HSLA Steel FANG Jian Abstract: Based on the determination of load variation against deflection by means of Instrumented
More informationPhase Transformations
Vysoká škola báňská Technická univerzita Ostrava Phase Transformations Didactic Text Vlastimil Vodárek Ostrava 2013 Review: Prof. Dr. Ing. Jaroslav Sojka Description: Phase Transformations Author: Vlastimil
More informationLecture 3: Introduction to Diffusion
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 3: Introduction to Diffusion Mass transport in
More informationThermodynamic database of the phase diagrams in copper base alloy systems
Journal of Physics and Chemistry of Solids 66 (2005) 256 260 www.elsevier.com/locate/jpcs Thermodynamic database of the phase diagrams in copper base alloy systems C.P. Wang a, X.J. Liu b, M. Jiang b,
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121. Spring Semester 2008 Professor R.
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationPhase Equilibria & Phase Diagrams
Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationHeat Treating Aluminum Alloys. Any sufficiently advanced technology is indistinguishable from magic Arthur C Clarke
Heat Treating Aluminum Alloys Any sufficiently advanced technology is indistinguishable from magic Arthur C Clarke Disclaimer This information is provided asis/whereis with no warranty expressed or implied.
More informationSome Data. Iron & Steel 61 Non ferrous 9.5 Plastics 11.5 Glass 3.0 Rubber 5.0 Other 10.0 Total weight / kg 901
Some Data Mg Al Ti Fe Density / g cm 3 1.74 2.7 4.51 7.87 Modulus / GPa 45 70 120 210 Specific Modulus / GPa cm 3 g 1 25.9 26 26 27 Melting Temperature / C 650 660 1670 1535 Crystal Structure (300 K) h.c.p.
More informationInterfacial Stress, Interfacial Energy, and Phase Equilibria in Binary Alloys
Journal of Statistical Physics, Vol. 95, Nos. 56, 1999 Interfacial Stress, Interfacial Energy, and Phase Equilibria in Binary Alloys William C. Johnson 1 and P. W. Voorhees 2 Received August 20, 1998 A
More informationMaster's Programs. Applied Chemisty. Subject
Master's Programs Applied Chemisty Optional Advanced Seminar in Materials Science and Engineering I Advanced Seminar in Materials Science and Engineering II Special Project in Materials Science and Engineering
More informationA Method of Calculating the Thickness of a SolidLiquid Interface
A Method of Calculating the Thickness of a SolidLiquid Interface Michael R. Atkins September 15, 2010 Abstract Microstructural evolution is a phenomenon of paramount importance in various areas of industry;
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationLecture 1: Kinetics vs. Thermodynamics: different but related
Lecture 1: Kinetics vs. Thermodynamics: different but related Today s topics The basic concepts of Kinetics and Thermodynamics, and how to understand the difference and interrelationship between the two
More informationCrystallization and energy relations between states of matter
Crystallization and energy relations between states of matter This text is meant as background information about how undercooling happens, and how the latent heat of crystallization has to be released
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationPhysical methods Physical Methods. Atomization Gas Atomization Water Atomization Cyrogenics Liquid Atomization Centrifugal Atomization
Physical Methods Atomization Gas Atomization Water Atomization Cyrogenics Liquid Atomization Centrifugal Atomization Atomization Atomization is the most important production method for metal powders. The
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationChemical Synthesis. Overview. Chemical Synthesis of Nanocrystals. SelfAssembly of Nanocrystals. Example: Cu 146 Se 73 (PPh 3 ) 30
Chemical Synthesis Spontaneous organization of molecules into stable, structurally welldefined aggregates at the nanometer length scale. Overview The 1100 nm nanoscale length is in between traditional
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationThe grade layer Al 2 O 3 Pd as intermetallic diffusion barrier
The grade layer Al 2 O 3 Pd as intermetallic diffusion barrier Figure 613 H 2 permeance as a function of time for membrane C01F08 at 500, 550 and 600ºC Figure 614 Selectivity (H 2 /He), H 2 permeance
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationPHASE TRANSITIONS IN POLYMERIC AND MICELLAR SYSTEMS
PHASE TRANSITIONS IN POLYMERIC AND MICELLAR SYSTEMS Summer School on Neutron Scattering and Reflectometry NG3 SANS Team NIST Center for Neutron Research June 37, 008 ABSTRACT SmallAngle Neutron Scattering
More informationHeat Treating Copper Beryllium Parts
Heat Treating Copper Beryllium Parts Heat treating is key to the versatility of the copper beryllium alloy system. Unlike other copper base alloys which acquire their strength through cold work alone,
More informationA. Xray diffraction B. elemental analysis C. band gap energy measurement based on absorption of light D. none of the above
LED Review Questions 1. Consider two samples in the form of powders: sample A is a physical mixture comprising equal moles of pure Ge and pure Si; sample B is a solid solution of composition Si0.5Ge0.5.
More informationDevelopment of a Model for Wet Scrubbing of Carbon Dioxide by Chilled Ammonia
Development of a Model for Wet Scrubbing of Carbon Dioxide by Chilled Ammonia John Nilsson Department of Chemical Engineering, Lund University, P. O. Box 124, SE221 00 Lund, Sweden In this paper, the
More information3.003 Lab 4 Simulation of Solar Cells
Mar. 9, 2010 Due Mar. 29, 2010 3.003 Lab 4 Simulation of Solar Cells Objective: To design a silicon solar cell by simulation. The design parameters to be varied in this lab are doping levels of the substrate
More informationPrecipitation hardening of a highly oversaturated Al4Zr solid solution
Precipitation hardening of a highly oversaturated Al4Zr solid solution R. von Bargen, J. Kovac, A. von Hehl, H.W. Zoch Lightweight Materials, IWT  Stiftung Institut für Werkstofftechnik, Germany 1 Introduction
More informationPhase. Gibbs Phase rule
Phase diagrams Phase A phase can be defined as a physically distinct and chemically homogeneous portion of a system that has a particular chemical composition and structure. Water in liquid or vapor state
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationCatalytic Nanoparticles in Solid Oxide Fuel Cells based on Triode Operation
Catalytic Nanoparticles in Solid Oxide Fuel Cells based on Triode Operation Vicky Broadley* and David Joyce Mantis Deposition, Ltd., Thame, UK Functional Thin Films meeting, 6 th Vacuum Expo 15 th October
More informationNPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] 1. Overview (C1) (Time: 49:06)
NPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] Lec Chapter 1. Overview (C1) (Time: 49:06) 2. Geometry of Crystals: Symmetry, Lattices (C2) (Time: 1:08:58) 3. (Time:
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationPrecipitation of carbides in Cr Mo V cast steel after service and regenerative heat treatment
ARCHIVES of FOUNDRY ENGINEERING Published quarterly as the organ of the Foundry Commission of the Polish Academy of Sciences ISSN (18973310) Volume 9 Issue 1/2009 97102 22/1 Precipitation of carbides
More informationELECD Principles of materials science Thermodynamics and diffusion. ELECD Principles of materials science
Thu 3.3 Mon 7.3 ELECD8710  Principles of materials science Thermodynamics and diffusion Thu 10.3 Exercise 5 Mon 14.3 Thu 17.3 Exercise 6 Mon 21.3 Thermodynamics  Principles (T,xi) equilibrium diagrams
More informationSolidification, Crystallization & Glass Transition
Solidification, Crystallization & Glass Transition Cooling the Melt solidification Crystallization versus Formation of Glass Parameters related to the formaton of glass Effect of cooling rate Glass transition
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationMaterial Strengthening Mechanisms. Academic Resource Center
Material Strengthening Mechanisms Academic Resource Center Agenda Definition of strengthening Strengthening mechanisms Grain size reduction Solid solution alloying Cold Working (strain hardening) Three
More informationThis is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th
More informationFormation of solids from solutions and melts
Formation of solids from solutions and melts Solids from a liquid phase. 1. The liquid has the same composition as the solid. Formed from the melt without any chemical transformation. Crystallization and
More informationThe Discussion of this exercise covers the following points:
Exercise 2 The Solar Panel (Photovoltaic Panel) EXERCISE OBJECTIVE When you have completed this exercise, you will be familiar with the operation of the silicon photovoltaic (PV) cell. You will be introduced
More informationIntroduction to microstructure
Introduction to microstructure 1.1 What is microstructure? When describing the structure of a material, we make a clear distinction between its crystal structure and its microstructure. The term crystal
More informationSOLIDIFICATION. (a)formation of stable nuclei. Growth of a stable nucleus. (c) Grain structure
SOLIDIFICATION Most metals are melted and then cast into semifinished or finished shape. Solidification of a metal can be divided into the following steps: Formation of a stable nucleus Growth of a stable
More information(i) outline the methods used by the Braggs to determine crystal structure
9.4.4 Investigations into the electrical properties of particular metals at different temperatures led to the identification of superconductivity and the exploration of possible applications 9.4.42(i)
More informationMonte Carlo Simulation technique. S. B. Santra Department of Physics Indian Institute of Technology Guwahati
Monte Carlo Simulation technique S. B. Santra Department of Physics Indian Institute of Technology Guwahati What is Monte Carlo (MC)? Introduction Monte Carlo method is a common name for a wide variety
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationCORROSIVE INFLUENCE OF MOLTEN MIXTURE OF
CORROSIVE INFLUENCE OF MOLTEN MIXTURE OF  ON INTERMETALLIC COMPOUND 3 Al IN THE PRESENCE OF MgO, ZnO, PbO, V 2 O 5, MoO 3 AND Fe 2 O 3 Aneta Magdziarz a Zofia Kalicka b a,b Faculty of Metallurgy and Materials
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationSolder Materials. Introduction
Solder Materials Introduction Most assemblies currently use solder in order to create connections between components and the printed circuit board. There was an indication in Polymer applications within
More informationMicroscale and Nanoscale Heat Transfer
Sebastian Volz (Ed.) Microscale and Nanoscale Heat Transfer With 144 Figures and 7 Tables In Collaboration with Remi Carminati, Patrice Chantrenne, Stefan Dilhaire, Severine Gomez, Nathalie Trannoy, and
More informationSimulation of diffusion controlled precipitation in heat treatable steels and its correlation with thermophysical properties
ThermoCalc user meeting, RWTH Aachen, 1.+2.9.2016 Simulation of diffusion controlled precipitation in heat treatable steels and its correlation with thermophysical properties S. Weber1, L. Mujica2, M.
More informationORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS
ORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS K. Sztwiertnia Polish Academy of Sciences, Institute of Metallurgy and Materials Science, 25 Reymonta St., 30059 Krakow, Poland MMN 2009
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationLecture 12: Heterogeneous Nucleation: a surface catalyzed process
Lecture 1: Heterogeneous Nucleation: a surface catalyzed process Today s topics What is heterogeneous nucleation? What implied in real practice of materials processing and phase transformation? Heterogeneous
More informationEstimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry
Estimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry Muhammed Olawale Hakeem AMUDA * and Raymond Otito AKABEKWA Department of Metallurgical and Materials Engineering
More informationIn the metals industry, there are numerous steps
How annealing, stress relief and aging each affect the mechanical properties of spring materials By Terry Bartel Elgiloy Specialty Metals In the metals industry, there are numerous steps from the raw material
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationThermal Analysis TGA / DTA. Linda Fröberg
Thermal Analysis TGA / DTA Linda Fröberg Outline Definitions What is thermal analysis? Instrumentation & origin of the TGADTA signal. TGA DTA Basics and applications Phase diagrams & Thermal analysis
More informationThermokinetics based materials modeling with MatCalc Functionality and integration
http://matcalc.at Thermokinetics based materials modeling with MatCalc Functionality and integration E. Kozeschnik Outline General information Thermodynamic engine Equilibrium and nonequilibrium thermodynamics
More informationFundamentals of Heat and Mass Transfer
2008 AGIInformation Management Consultants May be used for personal purporses only or by libraries associated to dandelon.com network. SIXTH EDITION Fundamentals of Heat and Mass Transfer FRANK P. INCROPERA
More informationSaturation Vapour Pressure above a Solution Droplet
Appendix C Saturation Vapour Pressure above a Solution Droplet In this appendix, the Köhler equation is derived. As in Appendix B, the theory summarised here can be found in Pruppacher & Klett (1980) and
More informationSection A5: Current Flow in Semiconductors
Section A5: Current Flow in Semiconductors Conductive behaviors in materials, defined by the parameter conductivity, are a primary factor in the development of electronic and optoelectronic devices. Electrical
More informationSolid State Detectors = SemiConductor based Detectors
Solid State Detectors = SemiConductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the pn junction Charge collection
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationKinetics of Phase Transformations: Nucleation & Growth
Kinetics of Phase Transformations: Nucleation & Growth Radhika Barua Department of Chemical Engineering Northeastern University Boston, MA USA Thermodynamics of Phase Transformation Northeastern University
More informationPh.D. Thesis Mohamed Fathy Hasaneen
Effect of Oxygen doping on Titanium Nitride thin films prepared by reactive unbalanced magnetron sputtering Ph.D. Thesis Mohamed Fathy Hasaneen Doctoral School of Physics Head: Prof. László Palla Doctoral
More informationKinetic Monte Carlo: from transition probabilities to transition rates
Kinetic Monte Carlo: from transition probabilities to transition rates With MD we can only reproduce the dynamics of the system for 100 ns. Slow thermallyactivated processes, such as diffusion, cannot
More information